SlideShare utilise les cookies pour améliorer les fonctionnalités et les performances, et également pour vous montrer des publicités pertinentes. Si vous continuez à naviguer sur ce site, vous acceptez l’utilisation de cookies. Consultez nos Conditions d’utilisation et notre Politique de confidentialité.
SlideShare utilise les cookies pour améliorer les fonctionnalités et les performances, et également pour vous montrer des publicités pertinentes. Si vous continuez à naviguer sur ce site, vous acceptez l’utilisation de cookies. Consultez notre Politique de confidentialité et nos Conditions d’utilisation pour en savoir plus.
WELDING INSPECTION - STEELS
THE DUTIES OF A WELDING INSPECTOR 9
CODES AND STANDARDS 12
THE WELDING PROCEDURE 14
DESTRUCTIVE TESTING 20
FOUR FACTORS FOR ESTABLISHING A WELD 37
RESIDUAL STRESS AND DISTORTION 44
HEAT TREATMENT 47
DEFECTS DETECTED BY SURFACE INSPECTION 50
INTERNAL DEFECTS 54
MACRO EXAMINATION 58
NON-DESTRUCTIVE TESTING 61
REPAIR BY WELDING 66
WELDING POSITIONS 75
MANUAL METAL ARC WELDING 78
TUNGSTEN INERT GAS WELDING 83
METAL INERT GAS WELDING 88
SUBMERGED ARC WELDING 94
AUTOMATIC METAL ARC WELDING 101
ELECTRON BEAM WELDING 103
ELECTRO-SLAG WELDING 105
Use of the correct terminology is important. CSWIP uses BS 499 standard. Frequently the terms
‘weld’ and ‘joint’ are used incorrectly. Exact definitions are given in BS 499 PT 1 1983 -
‘Welding terminology’ and BS 499 Pt 2: 1980 ‘ Weld symbols’.
TYPES OF WELD
At each weld
(Illustration depicts resistance weld.
Spot welds can be made with MIG
or TIG processes.)
The four basic welds can be used to join various types of joints.
TYPES OF JOINT
The following are some typical joints:
PLATE EDGE PREPARATION FOR BUTT WELDS
The illustrations show standard terminology for the various features of plate edge preparations.
Square edged closed butt Square edged open butt with backing strip
< 3 mm – sheet, > 3 mm - plate (considerations - penetration control, backing
strip of the same material and usually removed)
Backing bar - ceramic or copper Fusible insert - electric bolt (e.b)
(copper can cause loquation cracking) (Uses TIG process)
Single V Single bevel
Double V Double bevel
Single J Single U
Double J Double U
Bevel angle width
Root gap land
FEATURES OF A COMPLETED WELD
A butt weld in plate, made by welding from both sides, has two weld faces and four toes. In a full
penetration weld made from one side, the protruding weld on the underside is called the penetration
bead, which also has two toes. The root is defined (BS 499) as the zone on the side of the first run
farthest from the welder.
toe face toe
toe face toe
If a weld is sectioned, polished and etched, the fusion boundary can be established. Metal lying
between the two fusion boundaries is weld metal - a mixture of deposited metal and plate metal that
has been melted. The fusion zone is the area of highest dilution between filler metal and parent
plate. Adjacent to the fusion boundary is the heat affected zone (HAZ), in which the plate material
has had its metallurgical structure modified by the heat of welding.
Throat fusion boundary / line
Excess weld metal is the correct term, not ‘weld reinforcement’. Excess weld metal lying outside
the plane joining the toes of the weld.
Fillet welds have similar features.
The shape of a fillet in cross-section is described in three terms.
Mitre fillet Convex fillet Concave fillet
A convex fillet has a poor toe blend - greater notch effect and sharper angle at toe, not used in
fatigue situations. A concave fillet has a better toe blend for fatigue situations, however a reduced
throat. The concave weld may be made by welding alone or by subsequent grinding.
SIZE OF WELDS
Full Penetration Butt Welds.
The general rules are: design throat thickness = thickness of the thinner part joined.
Cap width = prep width + 10% either side (for open prep, not specified in BS
Partial Penetration Butt Welds.
The term partial penetration strictly implies butt welds that are designed to have less than full
penetration. Failure to achieve full penetration when it is wanted should be listed as the defect
The design throat thickness of a partial penetration weld is t1 and the actual throat thickness is t2.
With a partial penetration weld made from both sides, the design throat thickness is t1 + t1 and the
actual throat thickness is t2 + t2. Note that the degree of penetration must be known.
Fillet weld sizes are calculated by reference to allowable shear stress on the throat area, i.e.
Throat area = design throat thickness x length of weld.
The size required is specified on drawings in terms of leg length (l).
For fillet welds with equal leg lengths l = 1.4 t1. This does not apply to concave fillet welds.
l t1 = t2 t1 t1 t1 t1
If an asymmetrical weld is required, both leg lengths are specified and t1 is taken as the minimum
Deep penetration fillet weld.
With high current density processes, e.g. submerged arc and MIG (spray), penetration along the
joint line can be produced. This gives an increase in throat thickness with no change in leg length.
THE DUTIES OF THE WELDING INSPECTOR
At any point in the course of welding, i.e. tacking, root pass, filler pass or capping pass, but
particularly for the root and cap, a detailed inspection may be required. British Standard 5289: 1976
gives guidance on tools and responsibilities together with sketches of typical defects.
The inspector at this point must -
a) Observe, identify and perhaps record (measure) the features of the weld.
b) Decide whether the weld is acceptable in terms of the particular levels that are permitted;
defect levels may be ‘in-house’ or national codes of practice.
When the defect size is in excess of the permitted level then either a concession must be applied for
(from a competent person), or the weld rejected.
AIDS OF VISUAL INSPECTION
Illumination: Good lighting is essential.
Inspection Lenses: The magnification should not exceed 2 - 2.5 diameters. If higher
magnification is required use a binocular microscope.
Optical viewing can progressively develop from eyesight, to use of a hand torch and mirror, to the
addition of a magnifier and light source.
In order to achieve accessibility, remote probe units are available which must have the following
a) Large field of vision
b) Freedom from distortion of image
c) Accurate preservation of colour values
d) Adequacy of illumination
CODE OF PRACTICE
A code of practice for an inspection department should take the form outlined below. It is
appreciated that full implementation of the code would be extremely costly and therefore it may be
necessary to reduce the amount of inspection to less than is theoretically required.
The inspector should be familiar with the following:
a) All applicable documents
b) Workmanship standards
c) All phases of good workshop practice
d) Tools and measuring devices
INSPECTION BEFORE WELDING
Check * All applicable documents.
* Quality plan is authorised and endorsed with signature, date and company stamp.
* Application standard is up to date with the latest edition, revision or amendment.
* The drawings are clear, the issue number is marked and the latest revision is used.
* Welding procedure sheets (specifications) are available, have been approved and are
employed in production.
* Welder qualifications with identification and range of approval are verified and that only
approved welders as required are employed in production.
* Calibration certificates, material certificates (mill sheets) and consumer certificates are
available and valid.
* Parent material identification is verified against documentation and markings.
* Material composition, type and condition.
* Correct methods are applied for cutting and machining.
* Identification of welding consumables such as electrodes, filler wire, fluxes, shielding and
backing gases and any special requirements (e.g. drying) are met.
* Plant and equipment are in a safe condition and adequate for the job.
* Safety permits e.g. hot work permit, gas free permit, enclosed space certificate are
available and valid.
Check * Dimensions, tolerances, preparation, fit-up and alignment are in accordance with the
Approved drawings and standards.
* Tack welds, bridging pieces, clamping and type of backing - if any used are correct.
* Cleanliness of work area is maintained.
* Preheat in accordance with procedure.
NOTE Good inspection prior to welding can eliminate conditions that lead to the formation of
INSPECTION DURING WELDING
Check * the welding process must be monitored.
* Preheat and interpass temperatures must be monitored.
* Interpass cleaning - chipping, grinding, gouging, must be monitored.
* Root and subsequent run sequence.
* Essential variables such as current, voltage, travel speed to be monitored.
* Filler metals, fluxes and shielding gases are correct.
* Welding is in compliance with weld procedure sheet and application standard.
INSPECTION AFTER WELDING
Check * Visual inspection to be carried out to ascertain acceptability of appearance of welds.
* Dimensional accuracy to be ascertained.
* Conformity with drawings and standards requirements.
* Post weld heat treatment, if any, monitored and recorded.
* NDT carried out and reports assessed.
* Assess defects as to either repairing, or application for concession.
* Carry out any necessary repairs.
* Control of distortion
* Repair procedure and welding code should be authorised.
* Defect area should be marked positively and clearly.
* Check when partially removed and fully removed (visual and NDT).
* Re-welding should be monitored.
* Re-inspect completed repair.
Collate all documents and reports. Pass the document package on to a higher authority for final
inspection, approval and storage.
THE WELDING INSPECTOR
Ensure compliance with standard or code.
Ensure welding criteria by ‘policing’ work and documentation.
Honesty and integrity.
Fitness - physical and eyesight.
CODES AND STANDARDS
CLASS OF WORK
There are many types of work which require engineering materials to be joined by welding, for
Pressure vessels Bridges
Oil rigs Earth moving equipment
Aero-engines Ventilation systems
Storage tanks Heavy vehicle chassis
Car bodies Food processing plant
The quality requirements of the joints in these fabrications depend on their fitness-for-purpose and
differ significantly from one application to the next. Pressure vessels require welds, which can
withstand the stresses and high temperatures experienced in operation. Oilrigs are designed to
withstand the effect of wave formation and wind loads. Earth moving equipment has to
accommodate differences in terrain and earth conditions and is subject to fatigue loading. Welds in
food processing plants must withstand corrosion by hot acidic liquors.
Below are listed some typical codes of practice and standards which cover various types of
constructions fabricated by welding.
Code Class of Work
BS 5500 Unfired fusion welded pressure vessels
ASME VIII American boiler and pressure vessel code
BS 2633 Class 1 arc welding of ferritic steel pipe work for carrying fluids
BS 4515 Process of welding steel pipelines on land and offshore
BS 5950 Structural use of steelwork in building
AWS D1.1 Structural welding code (American)
BS 5400 Steel, concrete and composite bridges
BS 6235 Code of practice for fixed offshore structure
API 1104 Standard for welding pipelines and related structures
These documents can also provide a useful source of data for applications where codes do not exist.
It should be remembered, however, that the principal criterion in the codes listed is the quality of
the joint in relation to the service conditions. There are other applications where success is judged
by different criteria, such as dimensional accuracy.
Another important consideration is controlling the cost of welding. Variations in weld times and
quantities of consumables can readily result if the method of making a weld is left to the welder to
The continuous and satisfactory performance of weldments made to various codes requires that
specific guidelines are laid down to cover all variables. These guidelines are usually grouped under
the general heading of a Weld Procedure.
CODE OF PRACTICE
A code of practice is a set of rules for manufacturing a specific product. It should contain:
Design Requirements e.g. fit-up, preparation and type of joints
Materials e.g. types, thickness ranges
Manufacturer’s Working Practice
Inspection Criteria e.g. 100% visual, percentage other NDT
Acceptance Criteria e.g. defect size, limits, etc.
Welding Process e.g. type, consumables
Types of Tooling e.g. use of strong backs
The difference between a code and a standard is that a code states how to do a specific job and does
not contain all relevant information, but refers to other standards for details.
A code or standard generally mentions three parties - the customer or client, the manufacturer or
producer and the inspection authority. In a code the term ‘shall’ means mandatory - must be done,
and the term ‘should’ means recommended - not compulsory.
A concession is an agreement between the contracting parties to deviate from the original code
requirements. (BS 5135)
THE WELDING PROCEDURE
A welding procedure is a way of controlling the welding operation.
Purpose of procedure:
1) To prove a joint can meet design procedure - consistency
2) Instruction for welder
3) Ensure repeatability
Weld procedures are approved to ensure they are functional and fulfil the physical and mechanical
properties necessary to reach the required standard (to establish the essential variables for
Welders are approved to ensure a particular welder is capable of welding to a procedure and
obtaining a result that meets specification.
The task of collecting the data and drafting the documentation is often referred to as ‘writing’ a
weld procedure. In many ways this is an unfortunate term as the writing of documents is the last in a
sequence of tasks.
Producing a weld procedure involves;
Planning the tasks
Collecting the data
Writing a procedure for use or for trial
Making test welds
Evaluating the results of the tests
Approving the procedure of the relevant code
Preparing the documentation
In each code reference is made to how the procedures are to be devised and whether approval of
these procedures is required. In most codes approval is mandatory and tests to confirm the skill of
the welder are specified. Details are also given of acceptance criteria for the finished joint.
The approach used depends on the code, for example:
BS 2633 (Class 1 arc welding of ferritic steel pipe work for carrying fluids) provides general
comments on various aspects of a suitable weld procedure.
AWS D.1.1 (Structural welding code - steel) favours more specific instructions for different joints
and processes that are, in effect, pre-qualified procedures.
Other codes do not deal specifically with the details of the weld procedure but refer to published
documentation, e.g. BS 5135 ‘process of arc welding carbon and carbon manganese steels’.
COMPONENTS OF A WELD PROCEDURE
Items to be included in the procedure can be some of the following:
b. Thickness (for pipe this includes outside diameter)
c. Surface condition
d. Identifying marks
a. Type of process (MMA, TIG, SAW etc.)
c. Make, brand, type of welding consumables
d. When appropriate, the temperature and time adopted for drying and baking of electrodes
And / or consumables
a. Welding position
b. Edge preparation
c. Method of cleaning, degreasing etc.
d. Fit up of joint
e. Jigging or tacking procedure
f. Type of backing
a. Whether shop or site weld
b. Arrangement of runs and weld sequence
c. Filler material, composition and size (diameter)
d. Welding variables - voltage, current, travel speed
e. Weld size
f. Back gouging
g. Any specific features, e.g. heat input control, run-out length
a. Preheat and interpass temperatures including method and control
b. Post weld treatment including method and control
An essential variable is a variable that will influence or change the mechanical or metallurgical
properties of the welded joint - changes affecting the procedure approval. Any change in an
essential variable requires a new welding procedure specification (WPS).
Essential variables include: wall thickness, joint design, process, materials, consumables, welding
position, direction, heat input (voltage, amperage, and travel speed), heat treatment.
APPROVING THE PROCEDURE
When the data has been collected, the procedure must be validated by producing and testing a trail
If the procedure is to be used on a fabrication, which has been designed to meet the requirements of
a code, the test weld is done under the supervision of an independent witness. The detailed
arrangements for the test are subject to agreement between the contracting parties.
A number of British Standards make cross-reference to another standard which covers approval
testing. Other codes of practice include their own weld procedure / welder approval information. In
general they include a standard format, which can be used to report the results of an approval test.
Range of approval. (Extent of approval, scope of approval)
Provides a working range over which certain variables may alter without requiring a new welding
procedure or welder approval.
Variables include thickness (e.g. 1/2 down to 2x above), diameter (e.g. 1/2 down to 1/2 above)
materials (different materials can be covered), position, process, parent plate group, and
Re-approval of a welding procedure is necessary if there is a change of any of the essential
variables or considerable defect re-occurrence.
WPS welding procedure specification - an approved and accepted welding procedure; an
PQR procedure qualification records - proof the procedure works - record of tests
undertaken to qualify procedure.
WAC welder approval certificate - required to ensure a particular welder is capable of
welding to a procedure.
WATC welder approval test certificate.
WAR welder approval record.
WPAR welding procedure approval record.
WQT welder qualification test.
pWPS preliminary WPS - unauthorised (contains all essential variables and, after welding
the test piece and all NDT and destructive tests have been accepted, then the WPS
can be approved).
pWPS and WPAR give final WPS (various WPS can derive from one pWPS).
The objectives of a procedure or welder approval test are:
a. to prove the procedure meets the necessary requirements with reference to feasibility,
mechanical strength etc.
b. to prove the welders are competent to work on a particular job.
If a customer queries it, evidence can and would be supplied to prove validity.
Approval Test Specifications call for a paper record, which can be known as:
Procedure / welder approval certificate
Procedure / welder approval record
Procedure / welder approval report
The following records should also be kept:
Records of visual examination or mechanical testing
Test pieces from destructive testing
Other records that are equally important are proof of regular employment on a job for scheduling re-
tests to avoid duplication on procedure approval.
Welder approval tests are used to determine the ability of a welder to produce welds of an
acceptable quality with the processes, materials and welding positions that are to be used in
production. Dependant on the requirements and administration the manufacturer or contractor
may choose to qualify their own welders or they may employ outside personnel who can meet the
requirements. These requirements usually specify verification of the tests by an authorised inspector
or independent body. The requirements for the qualification of welders are usually laid down in the
governing code or specification or the contract specification.
Approval tests improve the probability of obtaining satisfactory welds in production. However it is
true to say that approval test welds are made with special attention and effort and so cannot show
whether or not the welder can do so under every production condition. For these reasons complete
reliance should not be placed on these qualifications - production welds should be inspected
regularly to ensure that the standard is being kept up.
Types of Approval Tests.
Tests that are prescribed by most codes and standards are in the main similar. Common tests are:
a. Plate and structural members.
b. Pipe welding.
c. Positions of welding.
d. Testing of approval test pieces.
a. Plate and structural members.
The requirements for welders of plate and structural parts (including pressure vessels) usually
require the welder to make one or more test welds on plate or pipe assemblies with the qualified
welding procedure. Each weld is tested in a specific manner, often both destructively and non-
destructively. The requirements normally state the applicability of material thickness and welding
positions that will qualify for production work. Other details will cover joint type and direction of
welding when depositing vertical welds (vertically up or vertically down).
b. Pipe welding.
The requirements for the approval of welders for pipe welding differs from those for welding plate
and structural members chiefly in the type of test assemblies and test positions. As a rule the welds
must be made on pipe and not plate. In some cases the space within which the test piece must be
welded may be restricted if the production work involves welding in cramped conditions. As
general rule welders who qualify for certain joints on pipe need not qualify for plate work, but
qualifications on plate do not apply to pipe work.
c. Position of welding.
Approval tests are normally expected to be made in the most difficult positions that will be
encountered in production welding. For example qualification in the vertical, horizontal and
overhead positions usually qualifies for welding in the flat position.
d. Testing of welder approval test pieces.
All codes and specifications will have definite rules for the testing of approval welds to determine
compliance. Most frequently this involves the removal of specimens for mechanical tests, such as
bend tests, and specimens for macro examination from specific locations in the test pieces. Non-
destructive testing may be required in conjunction with the mechanical tests.
Other properties required of the procedure qualification welds such as tensile strength, hardness,
etc. are not generally specified in welder approval tests since these properties depend primarily on
the parent and filler materials used on procedure details that are beyond the individual welder's
Welders whose test welds meet the requirements are qualified to use the process and to weld with
the filler metals and procedures similar to those used in testing. It should be mentioned that a
welder who has successfully welded a procedure test specimen is not required to undergo an
approval test, unless the requirements of production welding are different from those of the
procedure in which he has qualified.
The circumstances for the re-testing of a welder include the following:
1. Failure of the initial test welds.
2. A significant change in welding procedure.
3. A welder has not been engaged in welding for an extended period. (Usually three months.)
4. There is reason to question the welder's ability.
5. Change of employment without the transfer of his approval certificates.
CHECK LIST FOR WELDER AND PROCEDURE APPROVAL
1. The test being carried out is the correct one required.
2. Welders are in possession of all relevant information concerning the test.
3. Test materials confirm in all respects to requirements.
4. Joint configuration and tolerances are correct.
5. Welding plant and consumables.
6. The welder's identification is clearly marked on the test piece.
7. Where it is specified for a root run to be stopped and restarted in a certain position, that this
Position is clearly marked.
8. In the case of joints welded in fixed positions the test piece is so fixed that it cannot be
9. All ancillary tools such as chipping hammers, wire brushes, grinders, etc. are available.
The tests should be carried out without interruption but with sufficient supervision to ensure that the
requirements are being complied with. Where welder approval is carried out in accordance with
ASME section IX it states that the person supervising the test may, if in his opinion he considers
that the welder will not meet the required standard, terminate the test at any time. If it is necessary
to apply this ruling, it is suggested that full reasons for termination be recorded. It is further
recommended that the test piece should also be kept for a short period as a means of backing up
If the test is to be supervised by a representative of an independent authority he should be given all
the relevant details of the testing required.
Where British standards are involved, they generally state that if the welder is of the opinion that
his first attempt may not pass any subsequent testing, he may withhold it and weld a second. In this
case it is the second test piece that is submitted for examination and the first one must be scrapped.
Should state clearly that it is a welder approval and not a procedure approval, and, depending on
the particular standard, should contain the following:
a. welder’s name and identity number
b. date of test
c. standard of code in full, e.g. British Standard 4872 PT 1: 1982
d. test piece details including material specification
e. equipment and consumable details
f. extent of approval
g. sketch of run sequence, preparation and dimensions
h. other factors, operating parameters etc.
i. the test results (visual, NDT, DT etc.)
k. witnessed by
l. test supervisor
Most standards give an example of a test certificate.
Signatures on certificates must be endorsed by company stamp.
Destructive tests on welded joints are usually made as part of the approval of a welding procedure
or a welder.
Commonly used destructive tests are:
The test pieces are cut from the test weld and their location is often specified in the standard. The
British standard for the testing of welds is BS 709: 1983 Methods of testing fusion welded joints
and weld metal in steel. The areas for test are shown below.
Test weld along centre of plate
Macro section tensile
Short transverse bend
Object: To determine the soundness of weld metal, heat affected zone and weld zone.
These tests may also be used to give some measure of the ductility of the weld zone.
It is not usual to use transverse and longitudinal bend tests for the same application.
Method: All specimens to be removed and prepared without causing significant distortion or
heating. The cap and root are ground flush. The specimen is bent by the movement
of a former of prescribed diameter, the relevant side of the specimen to be placed in
tension. Angle of bend and diameter of former should be as specified in the
1. Thickness of specimen
2. Direction of bend (root or face)
3. Angle of bend
4. Diameter of former
5. Appearance of joint after bending e.g. type and location of flaws
Root bend face bend
This side in tension for face bend
This side in tension for root bend R R R R
Surface in contact with former ground flat. .R = roller support F = former of specified radius
SIDE BEND TEST
Object: To determine the soundness of the weld metal and HAZ in a cross section. This may
be preferred to the transverse bend test on thick materials. It is also used on
processes or procedures expecting lack of fusion (e.g. thick plate using MIG).
Method: The testing method is the same as that used for transverse bends except the cap and
root is not ground flush, to allow testing across the complete weld.
1. Width and thickness of specimen.
2. Angle of bend.
3. Diameter of former.
4. Appearance of joint after bending e.g. type and location of flaws.
This side in tension for R = roller support
Side bend F = former of specified radius
TRANSVERSE TENSILE TEST
Object: Used to measure the transverse tensile strength under static loading of a butt joint
employing butt welds.
The reduced section tensile test normally fails in the parent metal and so it is not
designed to give the tensile strength of the weld.
The radius reduced tensile test is a test of the as deposited diluted weld metal.
The all weld tensile test, using a longitudinal section from the weld only, is used to
check the as deposited undiluted weld metal. (Usually used by consumable
Method: The test piece is clamped at each end and a load is applied by a hydraulic or screw
Mechanism. The load is increased until fracture occurs.
1. Type of specimen (e.g. reduced section).
2. Whether excess weld metal is removed or not.
3. Tensile strength, in Newton's per mm squared, is calculated from maximum load and
original cross sectional area. When excess weld metal is not removed, the cross
sectional area shall be the product of the parent metal thickness and the width of the
4. Location of fracture - whether in parent plate, heat affected zone or weld metal. If
the fracture is in the parent metal, the distance from the weld zone shall be stated.
5. Location and type of any flaws present on the fracture surface.
Notch in weld
Reduced section tensile test radius reduced tensile test
The test gives a measure of percentage elongation, percentage reduction in area and ultimate tensile
UTS (yield stress strength point)
UTS = ultimate tensile strength
The tensile test gives a measure of DUCTILITY.
(In Newton's per mm squared a combination of percentage elongation and percentage reduction in
Types of failures.
Brittle fracture is flat and featureless.
Break Shear lips
A ductile fracture tears at 45° to the load.
IN-SERVICE BRITTLE FRACTURE
A flat surface with chevron markings that point to the material defect that initiated the fracture.
A flat surface with noticeable curves.
CHARPY V NOTCH IMPACT TEST
Object: To determine the amount of energy absorbed in fracturing a standardised testpiece at
a specified temperature.
Method: A machined, notched specimen is broken by one blow from a pendulum. Because
scatter occurs in the results, at least three specimens are used to assess the joint
Testing is carried out at a temperature specified in the appropriate application
The British standard is BS 131: PT 2: 1972.
1. Location and orientation of the notch.
2. Testing temperature.
3. Energy absorbed in joules.
4. Description of fracture appearance.
5. Location of any defects.
Hammer blow from this side
10mm p A
root radius a - anvil
0.25 mm t - test piece
h - Hammer
d - Dial calibrated in joules
p - Point reached after fracture
2 mm Energy absorbed during fracture
45° is proportional to (A - B)
CHARPY TEST PIECE CHARPY IMPACT MACHINE
The Charpy impact test, measured in joules, is an assessment of TOUGHNESS.
Transition temperature (curve) in steel. Ductile Failure
Brittle Failure (higher toughness )
FILLET WELD FRACTURE TEST
Object: To break the joint through the weld to permit examination of the fracture surfaces
for flaws and to check root penetration and fusion.
Method: The specimen is cut to length and a saw cut, normally 2 mm deep, is made along the
centre of the weld face. The specimen is fractured by bending or hammer blows.
1. Thickness of parent material.
2. Throat thickness and leg length.
3. Location of fracture.
4. Appearance of joint after fracture.
5. Depth of penetration / lack of penetration or fusion.
Hammer or bend saw cut
‘NICK’ BREAK (BEND) TEST
Object: As for fillet weld fracture, used on butt welds.
Method: The specimen is cut transversely to the weld, and a saw cut is applied along the
centre of the weld face. The best place for the cut is at a start / stop. The specimen is
fractured by bending or by hammer blows. The nick bend test will find internal
1. Thickness of material.
2. Width of specimen.
3. Location of fracture.
4. Appearance of joint after fracture.
Object: To examine a cross section of a weld for internal defects and soundness.
Method: A transverse section of the weld is cut out. The cross section is then visually
inspected. The section is filed down from rough to smooth, then emery or wet/dry
papered down to a surface finish of 600 grit. The surface is then etched in NITAL
(5% - 10% nitric acid in alcohol), washed off, rinsed and dried. (Possibly a final
clean with acetone and mount in Bakelite.) The specimen is then inspected at up to
2. Welding process.
3. Specimen identification.
4. Sentencing standard.
6. Geometric flaws - type, size and location.
7. Internal flaws - type, size and location.
8. Parent metal flaws - type, size and location.
9. Accept or reject, to standard, for each flaw.
Comparison of macro section and micro section:
Magnification X 10 X 1000
Finish 600 grit 1 micron (high level polish)
Features/defects cracks, slag, LOF, etc. intergranular structure
Uses procedure/welder qualification research/failure analysis
TYPES OF TEST
Quantitative (measurable) Qualitative
Tensile Bend test
Charpy Nick breaks
C.T.O.T. (crack tip opening test) Fillet fracture
Welds must be specified by clear instructions and all staff including production personnel must
understand the weld symbols specified.
It may be necessary to specify more details about the weld e.g. size, or electrode to be used, or even
the full details of a weld procedure may be needed.
The methods most commonly used to specify a weld are:
Weld XYZ is to be a single V butt welded from the outside of the vessel. The surface of the
weld is to be ground flush. The root is to be sealed with a weld run deposited from inside the vessel.
The completed weld is to be radiographed.
Symbols on a drawing:
Both the above give the same information.
Standards for weld symbols:
Although the main features of weld symbols are international, variations in detail occur from
country to country. Symbols are specified by national standards.
In this text symbols are in accordance with BSEN 22553, which supersedes BS 499 and is
identical to those in ISO 2553.
Indicating joint position:
An arrow indicates the position of the joint. The arrow points to one side of the joint. This is
called the ARROW SIDE. The side remote from the arrow is called the OTHER SIDE.
Arrow side other side arrow side
Information about the weld is given on a reference line attached to the arrow at a pivot. The
reference line is always horizontal and the arrow can swing about the pivot to point at the
weld. Details of the weld on the arrow side of the joint are given on the solid line. Other
side information is on the dotted line, which can be shown above or below the solid line.
Pivot reference line arrow side information
Other side information
A fillet weld is indicated by a triangle placed on the reference line.
A triangle on the reference line
Specifies a fillet weld on the =
Arrow side of the joint.
A triangle on the dotted line
Calls for a fillet weld on the =
Other side of the joint.-
TYPES OF BUTT WELD
The common types of edge preparation associated with a butt weld are indicated as follows:
Square edge preparation single V preparation
Double V preparation single U preparation
Using symbols it is not necessary to draw the
Double U preparation shape of the weld edge preparation. On any
Drawing the joint is always shown as a single
In some joints, only one component is prepared, e.g. single bevel butt or single J butt. In these
cases the arrow points at the edge which is to be prepared. The vertical upright of the symbol is
always to the left on the reference line.
DIMENSIONING FILLET WELDS
The leg length of a fillet weld is located to the left of the weld symbol (triangle). The dimension is
in millimetres preceded with the letter Z. Throat thickness is indicated in the same way but is
preceded by the letter a. If no letter is shown on a drawing, then assume the dimension is leg length.
Z 10 a 7
= 10 mm leg length = fillet weld with 7 mm
Fillet weld design throat
For deep penetration welds the dimensions are indicated e.g. S8 a6
This indicates a weld of 6 mm design throat, with an 8 mm
Actual throat desired. The actual throat thickness is
Proceeded by S.
Intermittent fillet welds are dimensioned by giving: Z n x l (e)
Number of weld elements (n)
Length of weld element (l)
Distance between weld elements (e)
Often the number of weld elements (n) is not specified, usually because it is not known.
The symbol can also be written as l (e) l, the length being repeated. The length is in centimetres.
A symbol thus z n x l (e) on a double fillet means the weld elements are to be
Staggered on either side of the joint.
Z 6 10(20) 10 6 mm throat fillet welds of 10 cm length with a gap of
= 20 cm between each element, staggered on either side
of the joint, for the whole joint’s length.
A compound weld is a combination of different welds on the same joint.
= A full penetration single bevel tee
Joint with 8 mm fillet reinforcement.
6 = an 8 mm partial penetration tee joint
With an 8 mm fillet reinforcement and
A 6 mm fillet on the other side of the
= A single V butt weld with a sealing run
along the root side of the weld.
The surface profile can be indicated by an extra symbol placed on top of the weld symbol.
= = a single V butt weld with a flat
Surface. (Usually flushed after
welding by grinding)
= a concave fillet weld.
= a convex fillet weld.
= a fillet weld with blended toes.
Other symbols in general use:
= weld all round the component.
= additional information. (the box on the tail of
the reference line can contain information e.g.
Weld process, NDT, paint, etc.)
= this weld welded on site. (Field weld)
= spot weld = seam weld
= plug weld = seal weld
= butt weld between plates with raised edges
In the older style, in BS 499 standard, the main difference was that there was no dotted reference
line, so below the reference line was the arrow side and above the reference line was the other side.
The term ‘steel’ is used to describe many different metals. They are all alloys based on iron, but the
alloying additions, such as carbon, manganese, silicon, chromium, etc., singly or in combination
produce a range of metals with widely differing physical and mechanical properties as well as quite
IRON Fe the basic constituent.
CARBON C gives hardness and strength.
MANGANESE Mn gives toughness and strength. Neutralises sulphur.
SILICON Si a deoxident - oxide reducer. Usually added through filler wire.
ALUMINIUM Al an oxide reducer, grain refiner and adds toughness. (In killed steel the
oxygen is removed by aluminium.)
CHROMIUM Cr gives corrosion resistance, high temperature strength and creep
resistance. (Grain creep occurs over time at high temperatures due to
MOLYBDENUM Mo gives high temperature creep resistance.
TITANIUM Ti Ti and Nb are both grain refiners and stabilising agents. They prevent
NIOBIUM Nb intergranular corrosion and weld decay. Used in austenitic steels.
VANADIUM V gives hardness and strength.
SULPHUR S a contaminant. (Main cause of solidification cracking - ‘hot
NICKEL Ni gives low temperature toughness and strength.
COPPER Cu a contaminant - causes liquation cracks. (Though also used for
weathering steel and a possible grain refiner.)
PHOSPHORUS P a contaminant.
Composition: 0.09% C 0.9% Mn + residuals
Weldability: The weld pool will require to have added deoxident via a filler rod.
Rimming steel is very ductile, cheap and used for pressing and forming. It is
low in carbon and high in oxygen - has not been killed (killed = deoxidised).
Low Carbon Steel
Composition: 0.2% C 0.9% Mn + residuals
Weldability: The general weldability is good but the level of residuals (S) may cause weld
metal / heat affected zone cracking.
Medium Carbon Steel
Composition: 0.45% C 0.9% Mn + residuals
Weldability: The high carbon content induces hydrogen cracking in the HAZ as the
section size increases. Greater than 0.38% C possibly requires heat treatment.
High Carbon Steel
Composition: 0.8% C 0.9% Mn + residuals
Weld-ability: The weld pool is subject to solidification type cracking and the HAZ
hydrogen cracking. Not suitable for welding. A tool steel.
Composition: 0.2% C 1.5% Mn + residuals may also contain Ti, Ni and V.
Weld-ability: These high manganese steels have good toughness, particularly the titanium,
niobium, and vanadium grades. The main weld-ability problem is to maintain
Quenched and Tempered Steel
Composition: 0.4% C 1.0% Mn 0.8% Cr 0.3% Mo + Ti or Al +
Weld-ability: These steels are difficult to weld, and defect free welds with good mechanical
properties are only obtained by using the greatest care.
High Temperature Steel
Composition: 0.25 - 9% Cr 0.25 - 3% Mo + traces
Weld-ability: The weld-ability of the low chromium is difficult. Good grain creep
Low Temperature Steel
Composition: 3.5 - 9% Ni + traces
Weld-ability: The higher nickel content is subject to solidification cracking.
Micro Alloyed Steel (HSLA)
Composition: 0.25% C 1.5% Mn (0.002% V, 0.005% Nb, 0.003% Ti minimum)
Weld-ability: These steels may suffer hydrogen cracking in the weld metal - the only weld
metal to do so. HSLA - High Strength Low Alloy.
Martensitic Stainless Steel
Composition: 11% Cr 0.08% C + residuals
Weldability: Poor due to hydrogen cracking.
Ferritic Stainless Steel
Composition: 12 - 27% Cr 0.08% C + residuals
Weld-ability: Poor due to cracking, brittleness and temper embrittlement.
Austinitic Stainless Steel
Composition: 18 - 27% Cr 8 - 22% Ni 0.08% C + residuals
Weld-ability: Problems with solidification cracking and weld decay - but does not suffer
hydrogen cracking. N.B. this is non-magnetic steel.
Carbon equivalency (C.E.) is used to give an overall carbon percentage to estimate the risk of
cracking. The higher the carbon content; the harder the steel - the more susceptible it is to cracking.
A carbon equivalency of 0.04% and above gives a greater risk of cracking.
C.E. = % C + % Mn + % Cr + Mo + V + % Ni + Co etc.
6 5 15
REVIEW OF STEELS
Types of steel used in welded constructions -
a. Low carbon - These steels are readily weld-able but may be subject to weld metal cracking
the cheaper qualities.
b. Medium carbon - As the carbon content approaches 0.4% steels become prone to parent
c. Low carbon/low alloy - The additional alloying elements acting in a similar way to carbon
again produce difficulties in welding.
d. High alloy steels - The austenitic stainless steels are prone to weld metal and reheat cracking
due to thermal conductivity characteristics.
The lower grades of constructional steel may exist in a number of forms due to the manufacturing
method used and these may exercise some influence on the weld-ability.
Rimming steel has not been deoxidised in the ingot mould and hence during solidification the
carbon reacts with the dissolved oxygen and is partly removed as carbon monoxide or dioxide. The
centre of the ingot solidifies with large quantities of oxygen entrapped, which may give rise to
porosity during welding.
Killed steel is deoxidised and although the resulting non-metallic inclusions may give rise to some
other problems porosity is not usually a prime problem.
Air blown acid or basic Bessemer steel will contain nitrogen, which lowers the impact properties
due to precipitation of FeN needles. This is becoming less of a problem with the advent of tonnage
oxygen and the basic oxygen process in steelmaking.
Deoxidants are varied but aluminium, silicon and manganese are widely used. Aluminium gives the
finer grain size, and hence a harder steel. However the fine grain size is lost when temperatures in
excess of 350°C are encountered.
Defects in parent materials. -
Many defects that arise in welding are directly due to the quality of the parent plate.
The specified composition plate material is not always achieved in all plates supplied. This is
because the composition of the steel in the ladle is changing with time but all the steel cannot be
cast instantaneously. Consequently it is quite possible that a welding procedure that works for one
plate may not work for another.
A great number of defects are produced during pouring and solidification of the ingot and although
some of these may be removed during hot and cold working, others may be produced.
Ingot defects include: surface defects (scabs, laps, etc.), solidification cracks, segregations,
inclusions, piping and porosity.
Rolling defects include: cracking and fishtail.
In the plate the most troublesome defects are: laminations, segregations or banding, cracks, porosity
A great variety of materials may require to be inspected with a view to satisfactory welding. The
main topics in material inspection are Size, Type and Condition.
It is not, in general, safe for the inspector to identify materials by composition from a mill
sheet, since very small variations or additions to the metal may give rise to significant
changes in properties and weldability. However limited selectivity is permissible, such as
percentage carbon maximum etc. The procedure is for the mill sheet to be submitted for
approval and then the inspector records and transfers the reference number.
This can be found on the Goods Inwards documents or the receipt documents, or
occasionally on packaging or even marked on the metal.
The quantity being inspected should always be noted as well as the sample size if 100 %
inspection is not being employed.
Sizes must be checked for secondary identification as well as conformance. The inspector
will, as appropriate, be given tolerances on size that are permissible. Check length, breadth,
thickness and diameter.
A check is often required on the degree of distortion, i.e.
Consistent wall thickness
Rust, paint and grease on the surface of the metal are all harmful to welding and must
usually be removed, at least near to the actual weld. Guidance is normally given to the
inspector regarding acceptable levels or the treatment that is required. An inspector should
be alert to gradual changes, such as increased corrosion. Carefully maintained specimens
showing acceptable conditions are often the best method. Heat treatment condition,
annealed, normalised etc., should all be recorded.
In wrought products the most common defects are laps and laminations (Also porosity and
segregation bands.) These will normally be subsurface so, unless NDE is employed, only the
edges of the plate, and particularly cut edges, can be inspected. The lap/lamination will
appear as a narrow black line parallel to the surface.
After inspection and approval for use it is essential that the metal is stored in such a way as
to maintain its good condition. Protect from corrosion and mechanical damage.
MATERIALS INSPECTION CHECK LIST
SIZE TYPE CONDITION
thickness composition physical mechanical
width carbon equivalent surface heat treatment
diameter trade name scale
ovality oil/grease annealed
flatness identification mark paint
quantity rust quench tempered
hard stamp/paint/etch thermo-mechanical
against mill sheet/
material certificate defects
tolerances? acceptable? acceptable?
ACCEPTANCE OF MATERIAL
QUESTIONS TO BE ASKED
1. Do the markings on the material match those on the procedure sheet or drawing?
2. Are the dimensions correct?
3. Is the surface condition satisfactory for welding?
THE FOUR ESSENTIAL FACTORS FOR ESTABLISHING A WELD
Welding is usually regarded as a joining process in which the work pieces are in atomic contact
often with a filler metal with broadly similar properties. Hence soldering and brazing are excluded
but both solid state and fusion welding are included.
Solid state processes include:
Fusion welding processes include:
Manual metal arc (MMA).
Metal inert/active gas (MIG/MAG).
Submerged arc welding (SAW).
Electro-slag welding (ESW).
FUSION WELDING FACTORS
1. Fusion. The metal must be melted which requires a high
intensity heat source.
2. Atmospheric protection. Contamination from the atmosphere must be avoided.
3. Surface protection. The process must remove any oxide and other
contamination from the joint faces.
4. Adequate properties. The welded joint must possess adequate mechanical,
metallurgical and physical properties.
Examples of the four factors:
TIG fusion source electric arc between wire and workplace.
atmospheric protection argon gas.
surface protection deoxidants in wire, mechanical cleaning.
properties from filler wire (possibly pre/post weld heat
MMA fusion source electric arc between electrode and workplace.
atmospheric protection gaseous shield from flux.
surface protection mechanical cleaning, slag, fluxing (cleaning) action.
properties alloying elements in flux, baking electrodes, pre and
post weld heat treatment.
As a result of the heat input to which the steel is exposed in any form of welding the material
undergoes certain changes, some of which are permanent. Amongst these changes are structural
transformations during heating and cooling and changes in shape or size due to the thermal stresses.
Steel, which can be welded without any dangerous consequences resulting from these changes, is
said to possess good weld-ability. If, on the other hand, the changes due to a normal welding
process are in serious danger of causing failure in a welded component, or if actual defects such as
cracking occur during welding, the steel is said to possess limited weld-ability and can in most cases
be welded, without risk, provided certain precautions are taken or certain pre- or post- welding
treatments are carried out. The term ‘un-weld-able steels’ is unrealistic. Any steel can be welded
provided correct metallurgical conditions are chosen. Sometimes, however, these conditions may be
impossible to realise in practical production work.
WELDABILITY OF STEEL
Weld-ability is a function of many inter-related factors but these may be summarised as:
1. Process and technique.
2. Composition of parent plate.
3. Joint design and size.
INFLUENCE OF PROCESS
Each process will give a characteristic intensity of power. Processes that offer the higher power
intensity offer advantages in fusion welding because the essential melting can be obtained without
excessive heat inputs with the consequent thermal expansion of the parent metal.
Successful welding often depends on feeding into the weld pool a filler wire which carries a
deoxidant (or ferrite forming elements) hence processes which do not use filler wire are limited in
Heat input is a combination of voltage, amperage and travel speed.
Heat Input = voltage x amperage
Heat Input 0.5 1 2 4
Hardness 475 450 300 275
(with hardness, the higher the number, the harder the material)
Toughness - resistance to bending and impact
Hardness - resistance to penetration
As heat input increases: grain size increases toughness decreases
brittleness increases hardness decreases
incidence of cracking decreases
There are four general factors that must be assessed to determine the level of preheat.
1. Material type.
2. Combined thickness.
3. Heat input potential (welding process).
4. Joint type.
INFLUENCE OF COMPOSITION
The composition of the steel and its effect on weld-ability may be divided into two parts:
1.Segregation effects, particularly that of sulphur.
When a steel solidifies, there is a tendency for the iron to solidify fast and for the alloying
elements to be accumulated in the centre of the ingot. This configuration is retained even after
prolonged and severe rolling and results in high concentrations of sulphur in the central layers of
the plate. These layers have little strength and are likely to crack if stressed.
2. The tendency of the steel to harden.
The hardening characteristics of steel are mentioned in the heat treatment section. As the
carbon or alloy content of the steel increases, the likelihood of low ductility and hardened
microstructures forming also increases and should stresses exist, cracking will result.
WELD AND HAZ CRACKING
These are the main causes of cracking:
a. High levels of carbon and other alloy elements result in brittle zones around the weld.
b. High cooling rates after welding increase the hardness, which increases the susceptibility to
c. Joint restraint prevents contraction after welding, which can lead to internal cracking.
d. Hydrogen in the weld bead can lead to hydrogen induced cold cracking.
e. Contaminants like sulphur and phosphorus cause segregation or solidification cracking.
f. Lamellar tearing caused by inclusions layering during rolling resulting in deterioration of
the through-thickness properties.
Cracking usually occurs in the unmelted areas adjacent to a weld bead (in the heat affected zone,
HAZ). This zone is made up of an area that has been heated to above about 800°C (to become
austenite), and an area heated above 723°C (and partially transformed). The fully austenitic region
just adjacent to the fusion zone is often the most brittle area of the weld due to the grain growth that
has occurred while the metal was at this temperature. The grain size gradually decreases moving
away from the fusion zone to the partially transformed region. Grain refinement occurs here,
which is considered beneficial, the grain size being smaller.
The composition of the steel, particularly the carbon level, determines the hardness and
brittleness of both the weld and the HAZ. On cooling, austenite transforms to ferrite. Carbon is
soluble in austenite, but less so in ferrite. Iron carbides are precipitated when this transformation
takes place. These can be arranged in lamellar form (as pearlite), which gives the structure
reasonable strength and ductility.
The HAZ can be the region where the highest cooling rates occur, particularly in thicker
section plate. High cooling rates tend to lock the carbides in a solid solution, forming martensite.
This leads to high internal stress and hard brittle structures.
TYPICAL WELDABILITY DEFECTS
1. SOLIDIFICATION CRACKING.
Also known as hot cracking or centreline cracking. Always occurs in the weld metal.
Causes - In carbon manganese steels; sulphur in the parent plate, shape of the weld, stress - always
During solidification the centre of the weld is the last to cool. Sulphur from the parent plate forms
iron sulphide with iron from the weld pool. The iron sulphide forms a thin liquid film on the grain
boundaries, which has a lower melting point than iron, so as the weld cools it is pushed towards the
centre of the weld. The iron sulphide has very little tensile strength, so as it cools, the weld is under
stress and cracking will result. Phosphorous contamination in the material can also cause
Avoidance - Reduce sulphur (check mill sheets for levels < 0.03 %).
Cleaning (no oil, grease etc.).
Add manganese to the parent plate via the filler wire (forms manganese sulphide that
melts cools at approximately the same temperature as steel. Manganese sulphide is
more discreet therefore less cracking.).
Reduce dilution by reducing the weld size.
Deep and narrow weld preparations are susceptible. As a weld cools, grains grow from the
extremities towards the centre of the weld. In a narrow prep, as the grains grow towards the centre,
they interfere with each other’s growth. This grain impingement causes voids between the grains
and cracking will result.
Avoidance - Wider weld preparation (increase the included angle and / or gap size).
2. HYDROGEN CRACKING.
Also known as under bead cracking, hard zone cracking and hydrogen induced cold cracking
(HICC). This phenomenon can occur during the welding of hardenable steels, and is normally a
HAZ phenomenon. Hydrogen is more soluble in austenite than ferrite - it can easily be picked up by
the weld metal. When ferrite is formed the hydrogen solubility decreases, and hydrogen diffuses to
the HAZ where it can contribute to crack propagation.
There are four factors involved in hydrogen cracking. Avoid one factor and hydrogen cracking will
1. hydrogen > 15 ml hydrogen per 100 mg weld metal
2. temperature < 350° C
3. hardness > 400 VPN (Vickers pyramid number)
4. stress > 50 % yield (cannot be measured so assume it is > 50 % yield)
1. Hydrogen a) parent material dried (free from moisture).
b) low hydrogen rods (baked to less than 5 ml per 100 mg).
c) use lower potential hydrogen process.
(hydrogen potential - electron < TIG < MIG/MAG < SAW, MMA (low H)
< MMA (rutile))
d) heat treatment (pre and post weld).
2. Temperature post weld heat treatment. (keep at a higher temperature as long as possible to
help hydrogen diffusion. NDT as late as possible - 72 hours.).
3. Hardness a) preheating (to reduce the cooling rate)
b) keep interpass temperature to a minimum
c) higher heat input (gives a larger grain size)
d) post weld heat treatment -tempers hard HAZ, removes H2, reduces stress
4. Stress a) joint design
b) fit up
c) distortion control
d) stress relieve treatment (pre and post weld)
On high micro alloy steels it may occur in the weld metal, otherwise only in the HAZ.
3. LAMELLAR TEARING.
A step like crack that occurs in thick section tee joints and closed corner joints.
has ‘step like’
Causes - Poor through thickness ductility in parent plate where high shrinkage strains (through
thickness stress) act through the plate thickness in combination with parent metal inclusions. The
inclusions can be lamellar inclusions, small micro inclusions or tramp elements. Only occurs on the
leg with stresses on the non-rolling direction / through thickness.
Avoidance - Joint design (use pre-formed tees, use open corners).
Use buttering layer (possibly more ductile and will take up some of the shrinkage).
Use Z grade steel (has been tested in the short transverse direction using a STRA test
- Short Transverse Reduction in Area).
pre formed tee open corner buttering
4. WELD DECAY IN AUSTENITIC STAINLESS STEELS
Occurs in the HAZ due to the precipitation of chromium carbides. In the 550° C - 850° C range, the
chromium leaches out of the grain and reacts with the carbon to form chromium carbides, due to the
chromium having a greater affinity for carbon. This results in a chromium deficiency in the grains.
The chromium is in the grains for corrosion resistance, so when the chromium is lost, decay
(‘rusting’) occurs very quickly. The longer a zone is in the temperature range of 550° C to 850° C
the greater the area is susceptible to decay. This temperature range is usually just off the weld.
Avoidance - Reduce carbon - Use low carbon rods for example 316 L. But low carbon reduces
strength, so a stabilised stainless steel could be used with high carbon content but
with titanium and niobium added. (Carbon has a greater affinity for titanium and
niobium therefore titanium and niobium carbides are produced instead of chromium
Lower heat input - less time in the 550° C - 850° C temperature range.
Quench cool - less time in the 550° C - 850° C temperature range.
Keep interpass temperature low.
The keyword is precipitation (of the chromium). The material is then said to be sensitised - put it in
seawater, it rusts.
WELDING OF CARBON STEEL
These steels are also known as carbon-manganese and plain carbon steels. They are usually
welded with mild steel consumables without problems, but the weldability decreases with
increasing carbon levels or C.E. (carbon equivalent) values.
The very low carbon steels (C < 0.15%) can produce porosity when welded at high speed.
This problem can be overcome by increasing the heat input.
Steels with carbon contents between 0.15% and 0.25% are preferred for welding, as they
rarely present weldability problems if the impurity levels are kept low. The steels with carbon levels
higher than 0.25% can be susceptible to cracking if other hardening elements like Mn and Si are
present in fairly high percentages. These steels are best welded with low hydrogen processes or
electrodes, and thick sections may require some pre-heating to reduce the cooling rate.
The high carbon steels are used for their wear resistance and hardness (for example tool
steels). They are generally very brittle and require pre-heating, interpass heating and post weld
stress relief to prevent cracking.
Most medium carbon steels require one or more of the above treatments depending on
carbon level and joint thickness. They are always welded with low hydrogen processes or
consumables and it is usual to perform a weldability test before production welding.
WELDING OF LOW ALLOY STEELS
The most common low alloy steels are the nickel steels, the carbon-molybdenum and the
Nickel from 2% to 5% in a 0.15% to 0.25% carbon steel provides a combination of high
strength and high toughness at low temperatures. If the carbon level is below 0.18% welding can be
done without pre-heat. Above this level, similar precautions to those recommended for medium
carbon steels should be adopted.
The carbon-molybdenum and chromium-molybdenum steels are used for high temperature
applications as they have high creep resistance and high strength. Below 0.18% carbon no pre-heat
is required, but thicker sections with higher carbon levels are hardenable in air and therefore crack
sensitive. For very high carbon levels (0.55%) where welding is not recommended, an austenitic
stainless steel consumable can sometimes be used. The weld will have more ductility and less
strength than the parent plate and will relieve some of the internal stress. The HAZ will still be
brittle, however, making pre-heat essential.
WELDING OF HIGH YIELD QUENCH AND TEMPERED STEELS
These steels have martensitic structures that are formed by heat treatment during
manufacture. One of the most common of these steels is HY80, which is used on submarine hulls.
The steels rely on relatively high cooling rates for the strong martensitic structures to form.
Strength can be lost if the cooling rate is too slow. Too high a cooling rate, however, can cause
weld cracking. Both the minimum pre-heat temperature and the maximum inter-pass temperature
have to be carefully controlled to achieve the correct structure without cracking. Matching
consumables are usually used. Weaving should be limited to a maximum of 15mm to keep the heat
WELDING OF HIGH STRENGTH LOW ALLOY STEELS
Most of these steels do not rely on heat treatment for their strength. They have ferritic
structures with low carbon levels (0.2% and less) and small amounts of alloying elements in
solution (Mn, Cr, Ti, V, Nb, N).
There are many different types with varying degrees of strength, toughness and corrosion
resistance. They usually have good weldability, but the high strength does make them more
susceptible to cracking than low carbon steel. High heat inputs are usually recommended and pre-
heating is sometimes required.
BS 5135 states that weld-ability is the ability of a material to be joined by most of the weld
processes and still maintain most of the physical/mechanical properties for which it was originally
Good weldability - low risk of HICC, but solidification cracking risk due to poor grain structure.
Limited weldability - may risk hardening effects through welding / cutting and HICC.
Lamellar tearing - poor through thickness ductility and plate defects.
Avoidance of the above risks should lead to an ‘acceptable’ weld.
RESIDUAL STRESS AND DISTORTION
Metals contract during solidification and subsequent cooling, but if this contraction is prevented or
inhibited, residual stresses will develop. During normal cooling smaller grains develop first towards
the edges of the weld and larger grains develop in the middle of the weld as it cools. Most material
products contain residual stresses, often up to yield point. Pipe products, for example, are usually
very highly stressed.
The tendency to develop residual stresses increases when the heating and cooling are localised. So
welding with its very localised heating and the presence of liquid and solid metal in contact can be
expected to induce very high levels of residual stresses.
Residual stresses are a combination of unequal expansion / contraction coupled with restraint.
Residual stresses can be difficult to measure with any real accuracy, but a rough guide is that when
the weld metal exceeds two cubic inches (fourteen cubic centimetres) then the total residual stress is
about yield point in magnitude.
Normal welds develop the following residual stresses:
a) along the weld - longitudinal residual stress.
b) across the weld - transverse residual stress.
c) through the weld - Short transverse residual stress.
Longitudinal Residual Stresses.
Consider the two plates A and B joined by the weld metal C. The weld metal and the HAZ want to
contract, but this is resisted by the plates. So the weld metal and the HAZ are pulled out (placed in
tension) and the plates are pulled in (placed in compression).
+ + Tension
This can be shown diagrammatically: - Compression
Transverse Residual Stresses.
c1 c2 c3
Again consider two plates A and B with weld metal C. In order to see how the stresses develop we
must look at the deposition of small lengths of weld C1, C2, C3 etc.
Assume that the plates A and B are not restrained. Length C1 will contract and draw the plates
together so the level of residual stresses across the joint will be very low. Length C2 will attempt to
contract but C1 will prevent this, so (roughly) C1 is placed in compression and C2 in tension.
Length C3 also attempts to contract but is now prevented by C2, which is placed in compression,
and C1 is pulled into tension. So we find there is a reversal of transverse residual stresses along the
joint. This pattern is similar for a multipass weld.
Short Transverse Residual Stresses.
A C B thickness
Again consider plates A and B joined by weld metal C. The effect is like that of the longitudinal
residual stresses if the weld is a single pass. For multipass welds the condition is more like the
transverse residual stresses and we find tensile stresses at the surface and compressive stresses at
Total Residual Stresses.
In practice the three directions in which the residual stresses develop combine to give a
resultant or total residual stress.
Effect of restraint.
For any given welded joint the level of residual stresses tends to increase as the restraint on
the joint increases.
Reducing restraint will reduce residual stress and reduce the chance of cracking.
The action of residual stresses in welded joints is to cause distortion.
Consider a simple weld with a single V preparation.
The following movements can be detected:
1. Contraction in the weld metal and HAZ along the length of the weld.
2. Bowing, due to the greater volume of metal at the top of the weld.
3. Peaking due to the V angle.
4. Ripple (in sheet) away from the weld.
5. Contraction in the weld metal and HAZ transverse to the weld.
Control of distortion is achieved in one or more of three main methods:
1.Presetting - so that the metal distorts into the required position.
2.Clamping - to prevent distortion, but this increases the level of residual stresses.
3.Welding sequence - i.e. balanced, for example backskip welding.
Other methods of distortion control include:
Change of prep to a more open prep (e.g. a U prep).
Lower heat input.
Many metals must be given heat treatment before and after welding. The inspector’s function is to
ensure that the treatment is given, and given correctly, to the details supplied.
Below are the types of heat treatment available. The temperatures mentioned are for steel.
Process Temperature Cooling Result
Annealing 920° C hold, furnace cool annealing is a recrystalisation
improves ductility (softens)
very slow cool decreases toughness
makes bending, etc. easier
lowers yield stress
Normalising 920° C hold, air cool increases toughness
improves mechanical properties
slow cool relieves internal stress
Quench, harden 920° C hold, quench cool hardens carbon steels
prevents carbide precipitation in
austenitic stainless steels
fast prevents temper brittleness
when (in oil or water) cooling after tempering
prepares metal for tempering
Temper 550° C - 700° C hold, air cool increases toughness of quenched
Stress Relief 550° C - 700° C hold, air cool relieves residual stresses by
reduces yield point
reduces hydrogen levels
slow improves stability during
prevents stress corrosion
Preheat for welding 50° C - 250° C hold
Hydrogen soak ≈ 150° C hold
Above 920° C the grain structure and size of grain structure are affected. Below 900° C the grain
structure is not affected. The soak time is related to thickness, usually one hour per 25 millimetres
thickness. Differing cooling rates give different properties to the metal, so the cool down rate is also
critical. (Possibly monitoring at a stand off from the weld being treated.) For preheating and
hydrogen soak oxy-acetylene is not to be used (too localised a heat source), propane is to be used.
MONITORING THE HEAT TREATMENT
The method and location of the heat treatment are important, for example in a workshop furnace or
on site using electroblanket (cooperheat type) equipment. The temperature is measured with
thermocouples and recorded on a chart. The main points are:
controlled heat rise
cool down rate to unrestricted
The last test is a hardness test after cooling.
temperature rise soak time cool down
Typical heat treatment chart recording.
The inspector should ensure that:
a) Equipment is as specified and calibrated.
b) Operators are qualified.
c) Procedure as specified is used.
i.e. method of application, rate of heating and cooling, maximum temperature, soak
(holding) time, temperature measurement.
d) All documentation and records are in order.
CALIBRATION OF WELDING EQUIPMENT
Instrumentation fitted to arc welding equipment often becomes inaccurate through neglect, damage,
wear etc. The presence of errors in the readings may remain unknown and their extent unchecked.
As a result, the values of the welding parameters indicated may well lie outside the working
tolerances. Consequently problems may be experienced in achieving the desired weld quality. A
significant level of defects may be predicted with consequential costs of reworking, repair or even
In high quality welding, regular checking of the parameters is there essential and should form a
mandatory part of inspection / quality control.
There are many different types of calibration equipment available, including ammeters, voltmeters
or equipment specifically designed to measure all the welding parameters.
Whatever the type of calibration piece used, they must also be calibrated for accurate measurement
- usually to a national standard. The British standard for calibrated measuring devices is NAMAS -
the National Measurement Scheme. The British standard for arc welding equipment is BS 7570.
Calibration is carried out on any equipment with a gauge; validation is carried out on equipment
CHECKLIST FOR CALIBRATING ARC WELDING EQUIPMENT
Welding Inspection necessarily involves checking that the correct welding/cutting process is being
used, that the equipment is in workable condition and that the welding parameters of amperes and
volts are being adhered to.
The main parameter controlling heat input and penetration. Check with ammeters for
inaccuracies, usually with tong testers generally anywhere, but preferably as close to the
torch as possible. Tolerance +/- 3 %.
Which is related to arc length and responsible for the weld bead profile. Check with
voltmeter (multimeter) across the electrical circuit for inaccuracies as close to the arc as
possible, but not on the return lead. Tolerance +/- 5 %.
Wire feed speed:
The most important parameter in MIG/MAG and SAW. It determines the welding current
being drawn to a) melt the wire and b) fuse the workpiece. Check with a stopwatch for 15 -
30 seconds or preferably with a tachogenerator for inconsistency and inaccuracies. The wire
feed speed is considered more accurate than amperage because it can be physically
Determines heat input and penetration.
mechanised - pre-set travel speed and check meter against distance travelled in one minute.
manual - check run out length.
In recent years more attention has been given to quality assurance in arc welding operations and in
many cases it is of paramount importance to ensure that the correct welding parameters are being
used in order to meet these requirements. Accurate calibration of equipment therefore is necessary
and ‘certificates of calibration’ are required for all equipment. i.e. welding equipment, measuring
equipment, storage ovens etc.
DEFECTS DETECTED BY SURFACE INSPECTION
Defects, which can be detected by visual inspection, can be grouped under five headings.
2. Surface irregularities.
3. Contour defects.
4. Root defects.
1. SURFACE CRACKS
A crack is a linear discontinuity produced by fracture. Cracks may be longitudinal,
transverse, edge, crater, centreline, fusion zone, underbead, weld metal or parent metal.
longitudinal, in the weld metal (centreline) longitudinal, in the parent plate
transverse crater (star cracking)
2. SURFACE IRREGULARITIES
An irregular groove at a toe of a run in the parent
metal or in previously deposited weld metal. If
created sub-surface it becomes a very effective
slag trap in the body of the weld. Undercut is
essentially a notch that in turn becomes a focal
point for stress loading, thereby reducing the fatigue
life of the joint.
Causes - current too high, voltage too high, travel
speed too high, electrode too small, electrode angle.
An imperfection at the toe or root of a weld caused by
caused by weld metal flowing on to the surface of the
parent plate without fusing to it.
Causes - slow travel speed, large electrode, tilt angle,
A depression due to shrinkage at the end of a run
where the source of heat was removed.
Causes - breaking the arc too quickly, too rapid
Stray globules of weld material, on parent plate outside the weld.
Causes - damp electrodes, too high voltage, too high current, flux missing.
Stray flash (stray arcing)
The damage on the parent material resulting from the accidental striking of an arc away
from the weld. A small volume of base material is melted when the arc is struck. This
molten pool is quenched due to the rapid diffusion of heat through the plate. This may lead
to the formation of a crater that lends itself to cracking, or a change in grain structure by
creating a martensitic or brittle grain structure in the area of the arc strike. These
discontinuities may lead to extensive cracking in service.
Causes - operator error.
3. CONTOUR DEFECTS
The profile of a finished weld may considerably affect performance of the joint under load
bearing conditions. Specifications normally include details of acceptable weld profiles to be
used as a guide.
(The ideal profile is to remove the cap and leave the weld flush with the adjacent surfaces.
This would increase the fatigue life of the joint by a factor of 3.)
Excess weld metal.
Also excess convexity, excess reinforcement.
Additional weld metal above the surface plane of the
parent material or greater than the desired throat on
Lack of fusion.
A continuous or intermittent groove along the side of
the weld with the original weld prep face still intact.
Causes - not enough runs, operator error.
Incompletely filled groove.
A continuous or intermittent channel in the surface of
the weld, running along its length, due to insufficient
weld material. The channel may be along the centre or
along one or both edges of the weld.
Causes - not enough runs - procedure error, electrode
too small. Also called insufficient throat.
Not a BS 499 term. (possibly under contour / toe
blend) Unevenly sized capping runs.
Causes - electrode type, arc voltage conditions, welder
Not a BS 499 term. Variation of leg length on a fillet
Causes - tilt angle, run sequence.
N.B. Unequal legs may be specified as part of the design -
in which case they are not defects.
4. ROOT DEFECTS
Incomplete root penetration.
Failure of weld metal to extend into the root of the weld.
Causes - poor weld prep, root gap too small, root face
too big, small included angle, heat input too low.
Lack of root fusion.
Lack of union at the root of a joint.
Causes - poor weld prep, uneven bevel, root face too
large, linear misalignment, cleaning.
Excess penetration bead.
Excess weld metal protruding through the root of a
fusion weld made from one side only.
Causes - high heat input, poor weld prep - large
Root concavity. (suck-back, underwashing)
A shallow groove which may occur in the root of a
Causes - purge pressure, wide root gap, and residual stresses
A shallow groove along each side of a penetration bead.
Causes - contraction of the metal along each side of the
bead while in the plastic condition.
Burnthrough. (melt through, blowthrough)
A localised collapse of the molten pool resulting in a
hole in the weld run.
Causes - excess penetration, excess heat input (usually
at the end of a run), localised weld prep variations.
Non-standard term. A local surface irregularity at
a weld restart.
Non-standard term. Misalignment between two
welded pieces such that their surface planes are not
parallel or at the intended angles.
A reduction in metal thickness caused by the removal
of the surface of a weld and adjacent areas to below
the surface of the parent metal.
Grooves on the surface of the parent metal or weld metal made by a grinding wheel or
An indentation in the surface of the parent metal or weld metal resulting from the
application of a tool, e.g. a chipping tool, in preparation or dressing.
An indentation in the surface of the parent metal or weld metal due to a hammer blow.
A surface irregularity due to the breaking off of temporary attachments.
An imperfection in the surface of the parent metal usually in the form of small depressions.
Lack of fusion. Lack of union in a weld. a. between weld metal and parent metal.
b. between parent metal and parent metal.
c. between weld metal and weld metal.
Lack of sidewall fusion. Lack of union between weld metal and parent metal at a side of a
Lack of inter-run fusion. Lack of union between adjacent runs of weld metal in a multi-run
Inclusion. Slag or other foreign matter entrapped during welding. The defect is
more irregular in shape than a gas pore.
Oxide inclusion. Metallic oxide entrapped during welding.
Tungsten inclusion. An inclusion of tungsten from the electrode during TIG welding.
Copper inclusion. An inclusion of copper due to the accidental melting of the contact
tube or nozzle in self adjusting or controlled arc welding or due to
pick up by contact between the copper nozzle and the molten panel
during TIG welding.
Puckering. The formation of an oxide covered weld run or bead with irregular
surfaces and with deeply entrained oxide films, which can occur when
materials forming refractory oxides (e.g. aluminium and its alloys) are
Porosity. A group of gas pores.
Elongated cavities. A string of gas pores situated parallel to the weld axis. (Linear
Blowhole. A cavity generally over 1.5mm in diameter formed by entrapped gas
during the solidification of molten metal.
Wormhole. An elongated or tubular cavity formed by entrapped gas during the
solidification of molten metal.
Porosity. Is the result of gas being entrapped within the solidifying weld metal. Porosity will
be present in a weld if the welding technique, materials used or condition of the weld
joint promotes gas formation. If the molten weld metal cools slowly and allows all
gas to rise to the surface before solidification, the weld would be virtually free of
Isolated or uniform porosity: The cause of this form of singular porosity is generally
faulty welding technique or defective material or both.
Cluster or group porosity: Is a localised group of pores that may result from
improper initiation or termination of the welding arc.
Linear porosity: Always forms a straight line along a run of weld and is caused by
gas evolving from contaminants.
Overlap. (Cold lap/roll over.) Usually caused by incorrect manipulation of welding procedures
i.e. low current combined with wrong travel speed. This defect can occur on the
fusion face as well as the cap run if the fusion face contains tightly adhering oxides.
(This would only be detected by NDT and probably interpreted as lack of fusion.)
Overlap may be defined as a surface connected discontinuity that forms a severe
mechanical notch parallel to the weld axis.
Tungsten Particles of tungsten trapped in the weld metal deposited with the TIG process.
Inclusion. Usually occurs when the operator dips the tungsten electrode tip into the molten
pool. A second reason for this defect, not generally recognised, is that if the
operating current is set too high the electrode tip will melt and droplets of tungsten
will be fired into the molten pool by the shielding gas.
SPECIFIC CAUSES AND REMEDIES.
Excessive hydrogen, nitrogen or Use low hydrogen welding process; filler metals
oxygen in welding atmosphere high in deoxidisers; increase shielding gas flow
High solidification rate Use preheat or increase heat input
Dirty base metal Clean joint faces and adjoining surfaces
Dirty filler wire Use specially cleaned and packaged filler wire
and store in a clean area
Improper arc length, welding current Change welding conditions and techniques
or electrode manipulation
Volatisation of zinc from brass Use copper-silicon filler metal; reduce heat input
Galvanised steel Use E7010 electrodes and manipulate the arc
heat to volatilise the galvanised zinc ahead of the
molten weld pool
Excessive moisture in electrode covering Use recommended procedures for baking and
or on joint surfaces storing electrodes; preheat the base metal
High sulphur base metal Use electrodes with basic slagging reactions
Failure to remove slag Clean surface and previous weld bead
Entrapment of refractory oxides Power wire brush the previous bead
Tungsten in the weld metal Avoid contact between the electrode and
workpiece; use larger electrode
Improper joint design Increase bevel angle of joint
Oxide inclusions Provide proper gas shielding
Weld metal cracking
Highly rigid joint Preheat; relieve residual stresses mechanically;
minimise shrinkage stresses using back step or
block welding sequence
Excessive dilution Change welding current and travel speed; weld
with covered electrode negative; butter the joint
faces prior to welding
Defective electrodes Change to new electrode; bake electrodes to
Poor fit-up Reduce root opening; build up the edges with
Small weld bead Increase electrode size; raise welding current;
reduce travel speed
High sulphur base metal Use filler metal low in sulphur
Angular distortion Change to balanced welding on both sides of joint
Crater cracking Fill crater before extinguishing the arc; use a
welding current decay device when terminating
the weld bead
Base metal cracking
Hydrogen in welding atmosphere Use low hydrogen welding process; preheat and
hold for two hours after welding or post weld heat
Hot cracking Use low heat input; deposit thin layers; change
Low ductility Use preheat; anneal the base metal
High residual stresses Redesign the weldment; change welding
sequence; apply intermediate stress relief heat
High hardenability Preheat; increase heat input; heat treat without
cooling to room temperature
Brittle phases in the microstructure Solution heat-treat prior to welding
This section covers the interpretation of internal defects and their reporting with regard to the
During interpretation it is necessary to identify associated defects.
Report 1. Incomplete root penetration and root fusion.
In the above sketch incomplete root penetration can be seen but, because of the loss of penetration,
incomplete root fusion is also present.
Planar defects such as incomplete sidewall, incomplete inter-run and incomplete root fusion are
very often associated with the presence of a non metallic inclusion, typically slag for MMA and
SAW and deoxidiser residue for MIG and TIG (ferritic steels).
In this example incomplete sidewall fusion is present. Because the defect also has width it can
largely be associated with a ‘silica’ inclusion.
report 1. Incomplete sidewall fusion with associated silica dioxide inclusion - add
The next sketch shows a root penetration / fusion defect caused because of either insufficient root
gap or no back gouging. On examination incomplete sidewall fusion has resulted because of poor
report 1. Incomplete root penetration and root fusion.
2. Incomplete sidewall fusion. *
3. Incomplete sidewall fusion. *
* Your judgement will be necessary in order to determine any associated inclusion.
As previously mentioned, slag and silica inclusions are associated with specific processes. With
regard to interpretation the inspector must confirm the welding process in order to make an accurate
assessment. This may be by reference to the welding procedure or by assessment of the weld face.
Slag inclusions will be clearly volumetric against silica inclusions that will have length and limited
Slag inclusions or silica inclusions?
report 1. Slag inclusion.
2. Silica inclusion. (incomplete interpass fusion may also be present)
In general terms, slag inclusions are non-uniform in their shape; also very often the slag is still
Gas inclusions, on the other hand, are generally uniform in their shape and are of a metallic
Gas inclusions (pores), porosity or solid inclusions?
report 1. Slag inclusion.
2. Elongated gas cavity. dimensions required.
3. Gas pore.
The inspector should report any parent metal defects - laps, laminations and segregation bands.
Parent metal defects.
Report 1. Laminations (straight and narrow).
2. Laminar inclusions (small, straight and narrow).
3. Laps (near surface of material).
4. Segregation bands (similar to lamination but lacks definite edges - hazy).
The report for the Macro should include:
Macro identification, material, welding process, sentencing standard.
All internal defects with type size and accept/reject.
All surface defects with type, size and accept/reject.
Geometric defects (e.g. misalignment) with type size and accept/reject.
Name, signature and date.
All defects should be arrowed and numbered on the report. For CSWIP the sentencing standard is
ISO 5817 level B (stringent).
NON DESTRUCTIVE TESTING
Type of operation:
Manual or mechanised.
Main unit comprising pulse generator, display oscilloscope, probe (chosen to suit
Mode of operation:
A pulse of electrical energy is fed to the probe in which a piezo-electric crystal
converts it to mechanical vibrations at an ultrasonic frequency. The vibrations are
transmitted (via a layer of grease to exclude the air) through the work. If they
encounter a defect some are reflected back to the probe, where they regenerate an
electrical signal. A cathode ray tube trace, started when the original signal is sent,
displays the reflected defect signal and from it time - indicating distance from probe,
and amplitude - indicating defect size, can be calculated.
Most metal except those with coarse or varying grain structure.
Typical welding applications.
Welds in thick wall vessels.
Welds with access to one side only.
Probe frequency 1 - 5MHz
Access Good (can be battery operated)
Thickness range 5 - 500mm
Minimum defect size 5mm wide
Immediate presentation of results.
Not necessary to evacuate personnel.
Can be battery powered.
Depth location of defects.
Trained and skilled operator needed.
No pictorial record.
Moderate care needed as for all electrical equipment.
MAGNETIC PARTICLE INSPECTION
Type of operation.
Manual or mechanised.
Power supply. Contacts or coil. Ultra-violet lamp (optional). Portable or fixed
Mode of operation.
The work is magnetised either by passing a current through it, or through a coil
surrounding it. Defects on or near the surface disrupt the magnetic field (unless they
are parallel to it). A magnetic particle fluid suspension is applied which concentrates
around the defects. The work is viewed either directly or by ultra-violet light using a
dye which fluoresces - i.e. emits visible light (this must be done where normal
lighting is subdued). After testing, work may be demagnetised if required.
Magnetic materials only - ferritic steels and some nickel alloys.
Current 500 - 10,000 Amps (AC or DC)
Supply load 1 - 100 kVA
Minimum defect size 0.025mm wide at surface
Testing time 10 - 80 seconds
Typical welding applications.
Rapid inspection of welded structural details.
Production rate inspection of small components.
Direct indication of defect location.
Initial inspection by unskilled labour.
Some indication of sub-surface defects but of low sensitivity.
Not critically dependent on surface condition.
No use for non-magnetic materials.
Defect detection critically dependent on alignment across magnetic field.
Sub-surface flaws require special procedures.
Moderate care needed in handling electrical equipment and flammable fluids.
Type of operation.
Static - development may be mechanised.
Radioactive isotope in storage container. Remote handling gear. Lightproof cassette.
Photographic development facilities. Darkroom and illuminator for assessment.
Mode of operation.
Gamma rays, similar to X-rays but of shorter wavelength, are emitted continuously
from the isotope. It cannot be ‘switched off’ so when not in use, it is kept in a heavy
storage container that absorbs radiation. They pass through the work to be inspected.
Parts of the work presenting less obstruction to gamma rays, such as cavities or
inclusions, allow increased exposure of the film. The film is developed to form a
radiograph with cavities or inclusions indicated by darker images. Section thickness
increases (such as weld) appear as less dense images.
Wavelength of radiation 0.001 - 0.015 nm
0.01 - 1 nm (1.25MeV - 80KeV)
Portability good (except for container)
Exposure time 1 second - 24 hours
Thickness range up to 250 mm
Minimum defect size 1% of thickness
Most weldable materials can be inspected.
Typical welding applications.
Panoramic exposure for small work.
Advantages, limitations, consumables and safety as for X-ray radiography.
Type of operation.
Static or transportable.
X-ray tube. Stand and control gear. Lightproof cassette. Photographic development
facilities. Dark room and illumination for assessment.
Mode of operation.
X-rays are emitted from the tube and pass through the work to be inspected. Parts
of the work presenting less obstruction to X-rays, such as cavities or inclusions,
allow increased exposure of the film. The film is developed to form a radiograph
with cavities or inclusions indicated by darker images. Section thickness increases
(such as weld under-bead) appear as less dense images.
Tube voltage 10 - 500 kV
Tube current 10 - 250 mA
Power consumption 1 - 10 kW
Exposure time 1 sec - 10 min
Thickness range up to 100 mm
Minimum defect size 0.1% of thickness X 0.05 mm
Most weldable materials may be inspected.
Typical welding applications.
Accurate pictorial presentation of results.
Radiographs may be kept as a permanent record.
Not confined to welds.
Personnel must be clear of area during exposure.
Cracks parallel to film may not show up.
Isotope replacements - for gamma radiography
Cumulative radiation risk to personnel requires stringent precautions.
DYE PENETRANT INSPECTION
Type of operation.
Manual or mechanised.
Minimum - aerosols containing dye, developer, cleaner.
Maximum - Tanks, work handling gear, ultra-violet lamp.
Mode of operation.
A special dye is applied to the surface of the article to be tested. A suitable time
interval allows it to soak into any surface defects. The surface is then freed from
surplus dye and the dye in the crack revealed by either: applying a white powder
developer into which the dye is absorbed producing a colour indication,
or, illuminating with ultra-violet light under which the dye fluoresces, that is, emits
visible light. This must be done where normal lighting is subdued.
Portability excellent (for aerosols)
Minimum defect size 0.025 mm wide
Time 30 minutes approx.
Any - non porous.
Typical welding applications.
Root runs in pipe butt welds.
Leak paths in containers.
Direct indication of defect location.
Initial examination by unskilled labour.
Surface defects only detected.
Defects cannot readily be rewelded due to trapped dye.
Rough welds produce spurious indications.
Dye and propellant gases have low flash points.